LMucko/crystallography-open-database huggingface dataset:
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1103 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003016
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1103 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5442
_cell_length_b                   8.5442
_cell_length_c                   8.5442
_cell_formula_units_Z            8
_cell_volume                     623.755
_database_code_amcsd             0003105
_diffrn_ambient_temperature      1376.15
_exptl_crystal_density_diffrn    3.418
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003016
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1167 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003017
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1167 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5519
_cell_length_b                   8.5519
_cell_length_c                   8.5519
_cell_formula_units_Z            8
_cell_volume                     625.443
_database_code_amcsd             0003106
_diffrn_ambient_temperature      1440.15
_exptl_crystal_density_diffrn    3.409
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003017
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1232 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003018
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1232 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5597
_cell_length_b                   8.5597
_cell_length_c                   8.5597
_cell_formula_units_Z            8
_cell_volume                     627.156
_database_code_amcsd             0003107
_diffrn_ambient_temperature      1505.15
_exptl_crystal_density_diffrn    3.399
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003018
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1297 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003019
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1297 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5674
_cell_length_b                   8.5674
_cell_length_c                   8.5674
_cell_formula_units_Z            8
_cell_volume                     628.850
_database_code_amcsd             0003108
_diffrn_ambient_temperature      1570.15
_exptl_crystal_density_diffrn    3.390
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003019
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1359 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003020
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1359 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5754
_cell_length_b                   8.5754
_cell_length_c                   8.5754
_cell_formula_units_Z            8
_cell_volume                     630.613
_database_code_amcsd             0003109
_diffrn_ambient_temperature      1632.15
_exptl_crystal_density_diffrn    3.381
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003020
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1403 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003021
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1403 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5814
_cell_length_b                   8.5814
_cell_length_c                   8.5814
_cell_formula_units_Z            8
_cell_volume                     631.938
_database_code_amcsd             0003110
_diffrn_ambient_temperature      1676.15
_exptl_crystal_density_diffrn    3.374
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003021
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1416 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003022
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1416 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5820
_cell_length_b                   8.5820
_cell_length_c                   8.5820
_cell_formula_units_Z            8
_cell_volume                     632.071
_database_code_amcsd             0003111
_diffrn_ambient_temperature      1689.15
_exptl_crystal_density_diffrn    3.373
_cod_original_cell_volume        632.070
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003022
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1397 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003023
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1397 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5807
_cell_length_b                   8.5807
_cell_length_c                   8.5807
_cell_formula_units_Z            8
_cell_volume                     631.783
_database_code_amcsd             0003112
_diffrn_ambient_temperature      1670.15
_exptl_crystal_density_diffrn    3.375
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003023
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1346 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003024
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1346 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5735
_cell_length_b                   8.5735
_cell_length_c                   8.5735
_cell_formula_units_Z            8
_cell_volume                     630.194
_database_code_amcsd             0003113
_diffrn_ambient_temperature      1619.15
_exptl_crystal_density_diffrn    3.383
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003024
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1283 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003025
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1283 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5661
_cell_length_b                   8.5661
_cell_length_c                   8.5661
_cell_formula_units_Z            8
_cell_volume                     628.564
_database_code_amcsd             0003114
_diffrn_ambient_temperature      1556.15
_exptl_crystal_density_diffrn    3.392
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003025
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1219 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003026
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1219 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5586
_cell_length_b                   8.5586
_cell_length_c                   8.5586
_cell_formula_units_Z            8
_cell_volume                     626.914
_database_code_amcsd             0003115
_diffrn_ambient_temperature      1492.15
_exptl_crystal_density_diffrn    3.401
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003026
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 1081 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003027
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 1081 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5413
_cell_length_b                   8.5413
_cell_length_c                   8.5413
_cell_formula_units_Z            8
_cell_volume                     623.120
_database_code_amcsd             0003116
_diffrn_ambient_temperature      1354.15
_exptl_crystal_density_diffrn    3.421
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003027
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 944 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003028
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 944 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5275
_cell_length_b                   8.5275
_cell_length_c                   8.5275
_cell_formula_units_Z            8
_cell_volume                     620.105
_database_code_amcsd             0003117
_diffrn_ambient_temperature      1217.15
_exptl_crystal_density_diffrn    3.438
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003028
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 882 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003029
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 882 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5199
_cell_length_b                   8.5199
_cell_length_c                   8.5199
_cell_formula_units_Z            8
_cell_volume                     618.448
_database_code_amcsd             0003118
_diffrn_ambient_temperature      1155.15
_exptl_crystal_density_diffrn    3.447
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003029
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 797 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003030
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 797 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5110
_cell_length_b                   8.5110
_cell_length_c                   8.5110
_cell_formula_units_Z            8
_cell_volume                     616.512
_database_code_amcsd             0003119
_diffrn_ambient_temperature      1070.15
_exptl_crystal_density_diffrn    3.458
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        '(Ti Mg2) O4'
_cod_database_code               9003030
An in situ neutron diffraction study of cation disordering in synthetic qandilite Mg2TiO4 at high temperature Sample: Second series, T = 756 C
O'Neill H St C; Redfern, S. A. T.; Kesson, S.; Short, S. M.; American Mineralogist 88 (2003) 860–865; doi:

data_9003031
_publ_section_title
;
 An in situ neutron diffraction study of cation disordering in synthetic
 qandilite Mg2TiO4 at high temperature
 Sample: Second series, T = 756 C
;
_journal_name_full               'American Mineralogist'
_journal_page_first              860
_journal_page_last               865
_journal_volume                  88
_journal_year                    2003
_chemical_formula_structural     Mg2(TiO4)
_chemical_formula_sum            'Mg2 O4 Ti'
_chemical_name_mineral           Qandilite
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.5075
_cell_length_b                   8.5075
_cell_length_c                   8.5075
_cell_formula_units_Z            8
_cell_volume                     615.752
_database_code_amcsd             0003120
_diffrn_ambient_temperature      1029.15
_exptl_crystal_density_diffrn    3.462
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Ti Mg2 O4'
_cod_database_code               9003031